state study no. 115 final report construction and testing of crumb rubber modified hot...
Post on 07-Jun-2020
Embed Size (px)
STATE STUDY NO. 115
CONSTRUCTION AND TESTING OF CRUMB RUBBER MODIFIED HOT MIX ASPHALT PAVEMENT
Gayle E. Albritton, PE William F. Barstis, PE
and Glynn R. Gatlin, PE
Research Division Mississippi Department of Transportation
In Cooperation with the
U. S. Department of Transportation Federal Highway Administration
Technical Report Documentation Page 1.Report No.
2. Government Accession No.
3. Recipient’s Catalog No.
5. Report Date
December 1999 4. Title and Subtitle
Final Report Construction and Testing of Crumb Rubber Modified Hot Mix Asphalt Pavement
6. Performing Organization Code
Gayle E. Albritton, William F. Barstis and Glynn R. Gatlin 8. Performing Organization Report No.
MS-DOT-RD-99-115 10. Work Unit No. (TRAIS)
9. Performing Organization Name and Address
Mississippi Department of Transportation Research Division P O Box 1850 Jackson MS 39215-1850
11. Contract or Grant No.
13. Type Report and Period Covered
12. Sponsoring Agency Name and Address
Federal Highway Administration
14. Sponsoring Agency Code
15. Supplementary Notes
16. Abstract This research project was structured toward addressing that portion of ISTEA which directs the individual states to conduct studies on the recyclability of crumb rubber modified (CRM) hot mix asphalt (HMA) and the technical performance of CRMHMA pavement. These objectives were addressed by monitoring the construction of highway test sections in which CRMHMA was incorporated into the pavement structure, evaluating the performance of these sections and then cold milling and recycling this pavement material into new HMA through a hot mix asphalt plant. This project was constructed in two phases in which the CRMHMA pavement was built in the first phase and approximately two years later milled and used as RAP in the surface course during the second phase. This report covers both phases of the construction. Three test sections were constructed in the westbound lanes of Federal Aid Project No. NH-007-1(53) on US 72 in Alcorn County. This project involved the paving of two new lanes that carried the westbound traffic of this route. The new lanes were paved and then placed under two-way traffic while old bridges were replaced on the old lanes. When the bridge construction was completed and the new lanes were carrying only westbound traffic, the surface course containing CRMHMA reclaimed asphalt pavement (RAP) was placed on the test sections. Primary conclusions and recommendations resulting from this study include the following: 1. During laboratory testing for the CRMHMA mix design, it was determined that the mixing temperature should be within the range of 351 to 390 degrees F.
2. The CRMHMA was successfully produced in a normal HMA production facility with the addition of a blending unit being the only modification to the HMA production process. 3. Some additional air pollution was visually observed when the CRM was mixed with the AC in the portable blending unit and during plant operation for the production of the
CRMHMA. 4. Review existing procedures and/or develop new procedures to mix the CRM with the asphalt cement at the terminal, deliver the blend to the HMA plant and maintain the blend
at the HMA plant. 5. Placement of the CRMHMA on the roadway appeared to be in a normal fashion as it would be for regular HMA, except for increased smoke due to the higher temperatures
required for compaction of the stiffer mix. 6. Laboratory tests conducted during phase one construction displayed a difficulty in achieving the design air voids at the design asphalt cement content for the CRMHMA. 7. Some gumming of the various components of the plant including the coating unit through to the surge bins was observed due to the use of the rubber modifier in the mix. This
did not pose a significant problem regarding plant operations for the production of the HMA for this study. 8. Initial performance tests were conducted on the CRMHMA pavement soon after completion of phase one construction. The pavement had low roughness readings and high
skid values indicating that it was in an excellent initial condition. 9. There was an increase in the average skid number with increasing amounts of CRM in the mix for the CRMHMA pavement. 10. Develop a new study to investigate the trend observed in this study of increased skid number with increased amounts of CRM in the HMA mix. 11. During milling operations of the CRMHMA pavement no gumming was observed of the teeth on the milling machine due to the rubber content in the pavement.. 12. The CRM RAP material was fed into the counter flow drum plant, as would any other RAP material. 13. No additional air pollution was visually noted during plant production of HMA containing the RAP with CRM. 14. Overall the rutting experienced by the sections is minimal for the length of time monitoring was performed for the surface course of the test sections containing 15 percent
CRM RAP material or the control section containing 11 percent RAP material.
17. Key Words
Recycling, waste tires, crumb rubber modified hot mix asphalt pavement
18. Distribution Statement
19. Security Classif. (of this report)
Unclassified 20. Security Classif. (of this page)
Unclassified 21. No. of Pages
117 22. Price
Form DOT F 1700.7 (8-72)
Reproduction of completed page authorized
The contents of this report reflect the views of the authors, who are responsible for the facts and accuracy of the data presented herein. The contents do not necessarily reflect the views or policies of the Mississippi Department of Transportation or the Federal Highway Administration. This report does not constitute a standard, specification, or regulation.
This document is disseminated under the sponsorship of the Department of Transportation in the interest of information exchange. The United States Government and the State of Mississippi assume no liability for its contents or use thereof.
The United States Government and the State of Mississippi do not endorse products or manufacturers. Trade or manufacturers names appear solely because they are considered essential to the object of this report.
The study reported herein was conducted by the Mississippi Department of Transportation (MDOT) under the sponsorship of the Federal Highway Administration, Mississippi Division Office. The work was accomplished during the period May 1995 through October 1999 under the supervision of Mr. Alfred B. Crawley, State Research Engineer followed by Ms. Joy F. Portera, State Research Engineer. This report was prepared by Messrs. Gayle E. Albritton, William F. Barstis and the late Glynn R. Gatlin of the MDOT Research Division.
The authors wish to express their appreciation to the many people whose efforts contributed to this study. Acknowledgment is made to Messrs. Johnny Hart, Reginald Jenkins, Roger Tingle, and James Watkins of the Research Division for their support during the performance testing of the project and to Gary S. Browning for his support in preparing some of the graphs for this report. Additional acknowledgment is made to involved personnel in the First District of MDOT, the paving contractor, APAC Mississippi, and Rouse Rubber Industries, Inc.
During the period of this study, the Executive Director of MDOT was Dr. Robert L. Robinson followed by Mr. Kenneth I. Warren. The Deputy Executive Director/Chief Engineer was Mr. James D. Quin, Mr. Kenneth Warren and Mr. James Kopf, respectively.
TABLE OF CONTENTS
TABLE OF CONTENTS iv
LIST OF TABLES v
LIST OF FIGURES vi
EXECUTIVE SUMMARY ix
CHAPTER 1 INTRODUCTION 1 1.1 Background 1.2 Objectives 1.3 Scope
CHAPTER 2 DESIGN AND CONSTRUCTION 3 2.1 Mixture Designs 2.2 Asphalt Plant 2.3 Construction of Pavement
2.3.1 Base Preparation 2.3.2 Control Section 2.3.3 Test Sections
2.4 Cost Comparison
CHAPTER 3 TEST RESULTS AND DISCUSSION 47 3.1 Laboratory Tests During Construction 3.2 Performance Tests
CHAPTER 4 CONCLUSIONS AND RECOMMENDATIONS 69 4.1 Conclusions 4.2 Recommendations
APPENDIX A ASPHALT INSPECTORS DAILY REPORTS FOR PHASE ONE CONSTRUCTION 72
APPENDIX B ASPHALT INSPECTORS DAILY REPORTS FOR PHASE TWO CONTRUCTION 101
List of Tables
2.1 Bituminous hot mix design for binder - control section 11
2.2 Bituminous hot mix design for surface - control section 12
2.3 Bituminous hot mix design for binder - 8% CRM 13
2.4 Bituminous hot mix design for binder - 10% CRM 14
2.5 Bituminous hot mix design for binder - 12% CRM 15
2.6 Bituminous hot mix design for surface for binder - 8% CRM 16
2.7 Bituminous hot mix design for surface for binder - 10% CRM 17
2.8 Bituminous hot mix design for surface for binder - 12% CRM 18
2.9 Bituminous hot mix design for mix containing 15% of 8% modified rubber RAP 19
2.10 Bituminous hot mix design for mix containing 15% of 10% modified rubber RAP 20